# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mo_hjkz5986_0m
_database_code_depnum_ccdc_archive 'CCDC 2067913'
loop_
_audit_author_name
_audit_author_address
'Pingzhang Yu'
;Institute of Crystal Materials, Shandong University 
China
;
_audit_update_record             
;
2021-03-04 deposited with the CCDC.	2021-08-19 downloaded from the CCDC.
;
_audit_creation_method           
;
FinalCif by Daniel Kratzert, Freiburg 2019,
https://github.com/dkratzert/FinalCif
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_formula_sum            'B3 Ca4 Ho O10'
_chemical_formula_moiety         ?
_chemical_formula_weight         517.68
_chemical_melting_point          ?
_chemical_absolute_configuration ?
_space_group_crystal_system      monoclinic
_space_group_IT_number           8
_space_group_name_H-M_alt        'C m'
_space_group_name_Hall           'C -2y'
_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x, -y, z'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z'

_cell_length_a                   8.090(3)
_cell_length_b                   16.018(7)
_cell_length_c                   3.5317(14)
_cell_angle_alpha                90
_cell_angle_beta                 101.284(4)
_cell_angle_gamma                90
_cell_volume                     448.8(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    2452
_cell_measurement_theta_min      2.8655
_cell_measurement_theta_max      31.197
_exptl_crystal_description       block
_exptl_crystal_colour            ?
_exptl_crystal_recrystallization_method ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.831
_exptl_crystal_F_000             484
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_absorpt_coefficient_mu    11.143
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.0131
_exptl_absorpt_correction_T_max  0.0524
_exptl_absorpt_process_details   
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_absorpt_special_details   ?
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_special_details           ?
_diffrn_ambient_temperature      296(2)
_diffrn_ambient_environment      N~2~
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  'mirror optics'
_olex2_diffrn_ambient_temperature_device 'Oxford Cryostream 800'
_diffrn_radiation_probe          x-ray
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_type              'Incoatec I\ms'
_diffrn_source_voltage           50.0
_diffrn_source_current           0.6
_diffrn_detector                 CCD
_diffrn_detector_type            'Bruker APEXII'
_diffrn_detector_area_resol_mean 8.3
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker APEX2 QUAZAR'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_measurement_specimen_support 'MiTeGen micromount'
_diffrn_reflns_number            2324
_diffrn_reflns_av_unetI/netI     0.0642
_diffrn_reflns_av_R_equivalents  0.0412
_diffrn_reflns_theta_min         2.543
_diffrn_reflns_theta_max         31.322
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_limit_l_max       4
_diffrn_measured_fraction_theta_max 0.949
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.949
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.814
_diffrn_reflns_point_group_measured_fraction_full 0.896
_reflns_number_total             1232
_reflns_number_gt                1227
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.704
_reflns_Friedel_fraction_max     0.678
_reflns_Friedel_fraction_full    0.792
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
_computing_data_collection       
'Bruker BIS 2011.4.0.0/01-Apr-2011 && APEX2_2011.4-1'
_computing_cell_refinement       'SAINT V8.40B'
_computing_data_reduction        'SAINT V8.40B'
_computing_structure_solution    'SHELXTL XT 2018/2'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0340P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_number_reflns         1232
_refine_ls_number_parameters     92
_refine_ls_number_restraints     3
_refine_ls_R_factor_all          0.0292
_refine_ls_R_factor_gt           0.0291
_refine_ls_wR_factor_ref         0.0777
_refine_ls_wR_factor_gt          0.0777
_refine_ls_goodness_of_fit_ref   1.063
_refine_ls_restrained_S_all      1.062
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_diff_density_max         2.722
_refine_diff_density_min         -2.404
_refine_diff_density_rms         0.289
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_coef       0.023(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_Flack   0.03(3)
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ho2 Ho 0.44425(4) 0.500000 0.47716(5) 0.0123(2) Uani 0.875(3) 2 d S T P A 1
Ca2 Ca 0.44425(4) 0.500000 0.47716(5) 0.0123(2) Uani 0.125(3) 2 d S T P A 2
Ho1 Ho 0.08451(19) 0.38754(10) 0.8032(5) 0.0135(4) Uani 0.0623(15) 1 d . . P A
1
Ca1 Ca 0.08451(19) 0.38754(10) 0.8032(5) 0.0135(4) Uani 0.9377(15) 1 d . . P A
2
Ca3 Ca 0.7016(2) 0.68116(13) 0.1261(6) 0.0167(4) Uani 1 1 d . . . . .
B1 B 0.3908(13) 0.6952(7) 0.554(3) 0.0135(18) Uani 1 1 d . . . . .
O1 O 0.2699(18) 0.500000 0.893(4) 0.016(2) Uani 1 2 d S T P . .
B2 B 0.816(2) 0.500000 0.173(5) 0.014(2) Uani 1 2 d S T P A .
O2 O 0.6405(17) 0.500000 0.081(5) 0.021(3) Uani 1 2 d S T P . .
O3 O 0.5250(9) 0.6413(5) 0.551(2) 0.0171(14) Uani 1 1 d . . . . .
O4 O 0.7314(9) 0.8257(5) 0.359(2) 0.0187(14) Uani 1 1 d . . . . .
O5 O 0.9112(10) 0.7312(5) 0.750(2) 0.0192(14) Uani 1 1 d . . . . .
O6 O 0.9033(10) 0.5743(4) 0.225(2) 0.0181(14) Uani 1 1 d . . . . .


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ho2 O1 2.227(14) . ?
Ho2 O1 2.259(14) 1_554 ?
Ho2 O2 2.312(15) . ?
Ho2 O3 2.356(8) . ?
Ho2 O3 2.356(8) 2_565 ?
Ho2 O2 2.397(16) 1_556 ?
Ho2 Ho2 3.5317(14) 1_556 ?
Ho2 Ho2 3.5317(14) 1_554 ?
Ho2 Ho1 3.7884(19) 2_565 ?
Ho2 Ho1 3.7884(19) . ?
Ho2 Ho1 3.8300(19) 1_554 ?
Ho2 Ho1 3.8300(19) 2_564 ?
Ca2 O1 2.227(14) . ?
Ca2 O1 2.259(14) 1_554 ?
Ca2 O2 2.312(15) . ?
Ca2 O3 2.356(8) . ?
Ca2 O3 2.356(8) 2_565 ?
Ca2 O2 2.397(16) 1_556 ?
Ca2 B1 3.176(11) 2_565 ?
Ca2 B1 3.176(11) . ?
Ca2 Ca1 3.7884(19) . ?
Ca2 Ca3 3.912(2) . ?
Ca2 Ca3 3.912(2) 2_565 ?
Ca2 Ca3 4.017(2) 1_556 ?
Ho1 O4 2.310(8) 3_446 ?
Ho1 O1 2.326(9) . ?
Ho1 O5 2.348(7) 2_465 ?
Ho1 O6 2.350(8) 2_465 ?
Ho1 O4 2.363(8) 3_445 ?
Ho1 O6 2.365(8) 2_466 ?
Ho1 Ho1 3.5317(14) 1_556 ?
Ho1 Ho1 3.5317(14) 1_554 ?
Ho1 Ca3 3.564(3) 3_446 ?
Ho1 Ho1 3.603(3) 2_565 ?
Ho1 Ca3 3.673(3) 2_466 ?
Ho1 Ca3 3.691(3) 2_465 ?
Ca1 O4 2.310(8) 3_446 ?
Ca1 O1 2.326(9) . ?
Ca1 O5 2.348(7) 2_465 ?
Ca1 O6 2.350(8) 2_465 ?
Ca1 O4 2.363(8) 3_445 ?
Ca1 O6 2.365(8) 2_466 ?
Ca1 B1 3.087(10) 2_565 ?
Ca1 B2 3.280(14) 1_456 ?
Ca1 Ca3 3.564(3) 3_446 ?
Ca1 Ca3 3.673(3) 2_466 ?
Ca1 Ca3 3.691(3) 2_465 ?
Ca3 O3 2.331(8) 1_554 ?
Ca3 O6 2.344(8) . ?
Ca3 O3 2.354(8) . ?
Ca3 O4 2.454(8) . ?
Ca3 O5 2.481(8) 1_554 ?
Ca3 O5 2.630(8) . ?
Ca3 B1 2.764(11) 4_565 ?
Ca3 O5 2.834(8) 4_464 ?
Ca3 B1 2.910(11) 1_554 ?
Ca3 O2 2.943(3) . ?
Ca3 B2 3.042(5) . ?
Ca3 B1 3.184(11) . ?
B1 O5 1.362(13) 4_465 ?
B1 O4 1.379(13) 4_465 ?
B1 O3 1.389(13) . ?
B2 O6 1.375(10) . ?
B2 O6 1.375(10) 2_565 ?
B2 O2 1.40(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Ho2 O1 103.8(6) . 1_554 ?
O1 Ho2 O2 176.1(7) . . ?
O1 Ho2 O2 80.1(5) 1_554 . ?
O1 Ho2 O3 97.1(2) . . ?
O1 Ho2 O3 102.22(19) 1_554 . ?
O2 Ho2 O3 81.9(2) . . ?
O1 Ho2 O3 97.1(2) . 2_565 ?
O1 Ho2 O3 102.22(19) 1_554 2_565 ?
O2 Ho2 O3 81.9(2) . 2_565 ?
O3 Ho2 O3 147.7(4) . 2_565 ?
O1 Ho2 O2 78.9(5) . 1_556 ?
O1 Ho2 O2 177.3(6) 1_554 1_556 ?
O2 Ho2 O2 97.2(5) . 1_556 ?
O3 Ho2 O2 77.29(19) . 1_556 ?
O3 Ho2 O2 77.29(19) 2_565 1_556 ?
O1 Ho2 Ho2 38.4(4) . 1_556 ?
O1 Ho2 Ho2 142.2(4) 1_554 1_556 ?
O2 Ho2 Ho2 137.7(4) . 1_556 ?
O3 Ho2 Ho2 86.74(18) . 1_556 ?
O3 Ho2 Ho2 86.74(18) 2_565 1_556 ?
O2 Ho2 Ho2 40.5(3) 1_556 1_556 ?
O1 Ho2 Ho2 141.6(4) . 1_554 ?
O1 Ho2 Ho2 37.8(4) 1_554 1_554 ?
O2 Ho2 Ho2 42.3(4) . 1_554 ?
O3 Ho2 Ho2 93.26(18) . 1_554 ?
O3 Ho2 Ho2 93.26(18) 2_565 1_554 ?
O2 Ho2 Ho2 139.5(3) 1_556 1_554 ?
Ho2 Ho2 Ho2 180.000(11) 1_556 1_554 ?
O1 Ho2 Ho1 34.5(2) . 2_565 ?
O1 Ho2 Ho1 84.1(3) 1_554 2_565 ?
O2 Ho2 Ho1 147.47(18) . 2_565 ?
O3 Ho2 Ho1 73.88(18) . 2_565 ?
O3 Ho2 Ho1 129.48(18) 2_565 2_565 ?
O2 Ho2 Ho1 98.3(3) 1_556 2_565 ?
Ho2 Ho2 Ho1 62.98(3) 1_556 2_565 ?
Ho2 Ho2 Ho1 117.02(3) 1_554 2_565 ?
O1 Ho2 Ho1 34.5(2) . . ?
O1 Ho2 Ho1 84.1(3) 1_554 . ?
O2 Ho2 Ho1 147.47(18) . . ?
O3 Ho2 Ho1 129.48(18) . . ?
O3 Ho2 Ho1 73.87(18) 2_565 . ?
O2 Ho2 Ho1 98.3(3) 1_556 . ?
Ho2 Ho2 Ho1 62.98(3) 1_556 . ?
Ho2 Ho2 Ho1 117.02(3) 1_554 . ?
Ho1 Ho2 Ho1 56.78(5) 2_565 . ?
O1 Ho2 Ho1 84.7(3) . 1_554 ?
O1 Ho2 Ho1 33.89(19) 1_554 1_554 ?
O2 Ho2 Ho1 98.8(3) . 1_554 ?
O3 Ho2 Ho1 132.95(18) . 1_554 ?
O3 Ho2 Ho1 77.16(18) 2_565 1_554 ?
O2 Ho2 Ho1 147.51(16) 1_556 1_554 ?
Ho2 Ho2 Ho1 118.21(3) 1_556 1_554 ?
Ho2 Ho2 Ho1 61.78(3) 1_554 1_554 ?
Ho1 Ho2 Ho1 82.94(5) 2_565 1_554 ?
Ho1 Ho2 Ho1 55.23(3) . 1_554 ?
O1 Ho2 Ho1 84.7(3) . 2_564 ?
O1 Ho2 Ho1 33.89(19) 1_554 2_564 ?
O2 Ho2 Ho1 98.8(3) . 2_564 ?
O3 Ho2 Ho1 77.16(18) . 2_564 ?
O3 Ho2 Ho1 132.95(18) 2_565 2_564 ?
O2 Ho2 Ho1 147.51(16) 1_556 2_564 ?
Ho2 Ho2 Ho1 118.21(3) 1_556 2_564 ?
Ho2 Ho2 Ho1 61.78(3) 1_554 2_564 ?
Ho1 Ho2 Ho1 55.23(3) 2_565 2_564 ?
Ho1 Ho2 Ho1 82.94(5) . 2_564 ?
Ho1 Ho2 Ho1 56.11(5) 1_554 2_564 ?
O1 Ca2 O1 103.8(6) . 1_554 ?
O1 Ca2 O2 176.1(7) . . ?
O1 Ca2 O2 80.1(5) 1_554 . ?
O1 Ca2 O3 97.1(2) . . ?
O1 Ca2 O3 102.22(19) 1_554 . ?
O2 Ca2 O3 81.9(2) . . ?
O1 Ca2 O3 97.1(2) . 2_565 ?
O1 Ca2 O3 102.22(19) 1_554 2_565 ?
O2 Ca2 O3 81.9(2) . 2_565 ?
O3 Ca2 O3 147.7(4) . 2_565 ?
O1 Ca2 O2 78.9(5) . 1_556 ?
O1 Ca2 O2 177.3(6) 1_554 1_556 ?
O2 Ca2 O2 97.2(5) . 1_556 ?
O3 Ca2 O2 77.29(19) . 1_556 ?
O3 Ca2 O2 77.29(19) 2_565 1_556 ?
O1 Ca2 B1 80.18(19) . 2_565 ?
O1 Ca2 B1 90.4(2) 1_554 2_565 ?
O2 Ca2 B1 99.94(19) . 2_565 ?
O3 Ca2 B1 167.4(3) . 2_565 ?
O3 Ca2 B1 23.7(3) 2_565 2_565 ?
O2 Ca2 B1 90.1(2) 1_556 2_565 ?
O1 Ca2 B1 80.18(19) . . ?
O1 Ca2 B1 90.4(2) 1_554 . ?
O2 Ca2 B1 99.94(19) . . ?
O3 Ca2 B1 23.6(3) . . ?
O3 Ca2 B1 167.4(3) 2_565 . ?
O2 Ca2 B1 90.1(2) 1_556 . ?
B1 Ca2 B1 159.9(4) 2_565 . ?
O1 Ca2 Ca1 34.5(2) . . ?
O1 Ca2 Ca1 84.1(3) 1_554 . ?
O2 Ca2 Ca1 147.47(18) . . ?
O3 Ca2 Ca1 129.48(18) . . ?
O3 Ca2 Ca1 73.87(18) 2_565 . ?
O2 Ca2 Ca1 98.3(3) 1_556 . ?
B1 Ca2 Ca1 51.71(19) 2_565 . ?
B1 Ca2 Ca1 108.47(19) . . ?
O1 Ca2 Ca3 130.86(8) . . ?
O1 Ca2 Ca3 89.2(2) 1_554 . ?
O2 Ca2 Ca3 48.49(6) . . ?
O3 Ca2 Ca3 33.84(18) . . ?
O3 Ca2 Ca3 126.49(18) 2_565 . ?
O2 Ca2 Ca3 88.9(2) 1_556 . ?
B1 Ca2 Ca3 147.92(19) 2_565 . ?
B1 Ca2 Ca3 52.14(19) . . ?
Ca1 Ca2 Ca3 159.59(4) . . ?
O1 Ca2 Ca3 130.86(8) . 2_565 ?
O1 Ca2 Ca3 89.2(2) 1_554 2_565 ?
O2 Ca2 Ca3 48.49(6) . 2_565 ?
O3 Ca2 Ca3 126.49(18) . 2_565 ?
O3 Ca2 Ca3 33.84(18) 2_565 2_565 ?
O2 Ca2 Ca3 88.9(2) 1_556 2_565 ?
B1 Ca2 Ca3 52.14(19) 2_565 2_565 ?
B1 Ca2 Ca3 147.92(19) . 2_565 ?
Ca3 Ca2 Ca3 95.78(7) . 2_565 ?
O1 Ca2 Ca3 87.0(3) . 1_556 ?
O1 Ca2 Ca3 133.00(6) 1_554 1_556 ?
O2 Ca2 Ca3 90.3(3) . 1_556 ?
O3 Ca2 Ca3 30.82(18) . 1_556 ?
O3 Ca2 Ca3 121.93(18) 2_565 1_556 ?
O2 Ca2 Ca3 46.63(5) 1_556 1_556 ?
B1 Ca2 Ca3 136.6(2) 2_565 1_556 ?
B1 Ca2 Ca3 45.9(2) . 1_556 ?
Ca3 Ca2 Ca3 52.88(3) . 1_556 ?
Ca3 Ca2 Ca3 117.92(6) 2_565 1_556 ?
O4 Ho1 O1 90.3(4) 3_446 . ?
O4 Ho1 O5 85.4(3) 3_446 2_465 ?
O1 Ho1 O5 175.7(4) . 2_465 ?
O4 Ho1 O6 168.6(3) 3_446 2_465 ?
O1 Ho1 O6 101.1(4) . 2_465 ?
O5 Ho1 O6 83.2(3) 2_465 2_465 ?
O4 Ho1 O4 98.2(3) 3_446 3_445 ?
O1 Ho1 O4 91.2(4) . 3_445 ?
O5 Ho1 O4 88.7(3) 2_465 3_445 ?
O6 Ho1 O4 80.9(3) 2_465 3_445 ?
O4 Ho1 O6 81.7(3) 3_446 2_466 ?
O1 Ho1 O6 100.1(4) . 2_466 ?
O5 Ho1 O6 80.0(3) 2_465 2_466 ?
O6 Ho1 O6 97.0(3) 2_465 2_466 ?
O4 Ho1 O6 168.7(3) 3_445 2_466 ?
O4 Ho1 Ho1 41.46(19) 3_446 1_556 ?
O1 Ho1 Ho1 89.4(3) . 1_556 ?
O5 Ho1 Ho1 87.9(2) 2_465 1_556 ?
O6 Ho1 Ho1 138.34(19) 2_465 1_556 ?
O4 Ho1 Ho1 139.66(19) 3_445 1_556 ?
O6 Ho1 Ho1 41.34(19) 2_466 1_556 ?
O4 Ho1 Ho1 138.54(19) 3_446 1_554 ?
O1 Ho1 Ho1 90.6(3) . 1_554 ?
O5 Ho1 Ho1 92.2(2) 2_465 1_554 ?
O6 Ho1 Ho1 41.66(19) 2_465 1_554 ?
O4 Ho1 Ho1 40.35(19) 3_445 1_554 ?
O6 Ho1 Ho1 138.66(19) 2_466 1_554 ?
Ho1 Ho1 Ho1 180.0 1_556 1_554 ?
O4 Ho1 Ca3 43.12(19) 3_446 3_446 ?
O1 Ho1 Ca3 123.4(3) . 3_446 ?
O5 Ho1 Ca3 52.5(2) 2_465 3_446 ?
O6 Ho1 Ca3 126.95(19) 2_465 3_446 ?
O4 Ho1 Ca3 71.75(19) 3_445 3_446 ?
O6 Ho1 Ca3 101.37(19) 2_466 3_446 ?
Ho1 Ho1 Ca3 74.46(4) 1_556 3_446 ?
Ho1 Ho1 Ca3 105.54(4) 1_554 3_446 ?
O4 Ho1 Ho1 115.39(19) 3_446 2_565 ?
O1 Ho1 Ho1 39.2(3) . 2_565 ?
O5 Ho1 Ho1 144.1(2) 2_465 2_565 ?
O6 Ho1 Ho1 74.91(18) 2_465 2_565 ?
O4 Ho1 Ho1 114.78(19) 3_445 2_565 ?
O6 Ho1 Ho1 75.01(18) 2_466 2_565 ?
Ho1 Ho1 Ho1 89.999(1) 1_556 2_565 ?
Ho1 Ho1 Ho1 90.0 1_554 2_565 ?
Ca3 Ho1 Ho1 158.05(4) 3_446 2_565 ?
O4 Ho1 Ca3 86.1(2) 3_446 2_466 ?
O1 Ho1 Ca3 138.6(3) . 2_466 ?
O5 Ho1 Ca3 41.86(19) 2_465 2_466 ?
O6 Ho1 Ca3 85.8(2) 2_465 2_466 ?
O4 Ho1 Ca3 130.16(19) 3_445 2_466 ?
O6 Ho1 Ca3 38.54(19) 2_466 2_466 ?
Ho1 Ho1 Ca3 61.61(4) 1_556 2_466 ?
Ho1 Ho1 Ca3 118.39(4) 1_554 2_466 ?
Ca3 Ho1 Ca3 79.06(5) 3_446 2_466 ?
Ho1 Ho1 Ca3 107.43(4) 2_565 2_466 ?
O4 Ho1 Ca3 130.5(2) 3_446 2_465 ?
O1 Ho1 Ca3 139.2(3) . 2_465 ?
O5 Ho1 Ca3 45.2(2) 2_465 2_465 ?
O6 Ho1 Ca3 38.09(19) 2_465 2_465 ?
O4 Ho1 Ca3 84.98(19) 3_445 2_465 ?
O6 Ho1 Ca3 86.6(2) 2_466 2_465 ?
Ho1 Ho1 Ca3 118.92(4) 1_556 2_465 ?
Ho1 Ho1 Ca3 61.08(4) 1_554 2_465 ?
Ca3 Ho1 Ca3 93.87(5) 3_446 2_465 ?
Ho1 Ho1 Ca3 107.34(4) 2_565 2_465 ?
Ca3 Ho1 Ca3 57.32(4) 2_466 2_465 ?
O4 Ca1 O1 90.3(4) 3_446 . ?
O4 Ca1 O5 85.4(3) 3_446 2_465 ?
O1 Ca1 O5 175.7(4) . 2_465 ?
O4 Ca1 O6 168.6(3) 3_446 2_465 ?
O1 Ca1 O6 101.1(4) . 2_465 ?
O5 Ca1 O6 83.2(3) 2_465 2_465 ?
O4 Ca1 O4 98.2(3) 3_446 3_445 ?
O1 Ca1 O4 91.2(4) . 3_445 ?
O5 Ca1 O4 88.7(3) 2_465 3_445 ?
O6 Ca1 O4 80.9(3) 2_465 3_445 ?
O4 Ca1 O6 81.7(3) 3_446 2_466 ?
O1 Ca1 O6 100.1(4) . 2_466 ?
O5 Ca1 O6 80.0(3) 2_465 2_466 ?
O6 Ca1 O6 97.0(3) 2_465 2_466 ?
O4 Ca1 O6 168.7(3) 3_445 2_466 ?
O4 Ca1 B1 75.5(3) 3_446 2_565 ?
O1 Ca1 B1 80.8(4) . 2_565 ?
O5 Ca1 B1 97.4(3) 2_465 2_565 ?
O6 Ca1 B1 105.2(3) 2_465 2_565 ?
O4 Ca1 B1 25.1(3) 3_445 2_565 ?
O6 Ca1 B1 157.2(3) 2_466 2_565 ?
O4 Ca1 B2 99.6(3) 3_446 1_456 ?
O1 Ca1 B2 88.8(3) . 1_456 ?
O5 Ca1 B2 92.6(3) 2_465 1_456 ?
O6 Ca1 B2 81.6(3) 2_465 1_456 ?
O4 Ca1 B2 162.2(3) 3_445 1_456 ?
O6 Ca1 B2 21.3(3) 2_466 1_456 ?
B1 Ca1 B2 168.4(3) 2_565 1_456 ?
O4 Ca1 Ca3 43.12(19) 3_446 3_446 ?
O1 Ca1 Ca3 123.4(3) . 3_446 ?
O5 Ca1 Ca3 52.5(2) 2_465 3_446 ?
O6 Ca1 Ca3 126.95(19) 2_465 3_446 ?
O4 Ca1 Ca3 71.75(19) 3_445 3_446 ?
O6 Ca1 Ca3 101.37(19) 2_466 3_446 ?
B1 Ca1 Ca3 61.0(2) 2_565 3_446 ?
B2 Ca1 Ca3 122.5(2) 1_456 3_446 ?
O4 Ca1 Ca3 86.1(2) 3_446 2_466 ?
O1 Ca1 Ca3 138.6(3) . 2_466 ?
O5 Ca1 Ca3 41.86(19) 2_465 2_466 ?
O6 Ca1 Ca3 85.8(2) 2_465 2_466 ?
O4 Ca1 Ca3 130.16(19) 3_445 2_466 ?
O6 Ca1 Ca3 38.54(19) 2_466 2_466 ?
B1 Ca1 Ca3 137.1(2) 2_565 2_466 ?
B2 Ca1 Ca3 51.51(17) 1_456 2_466 ?
Ca3 Ca1 Ca3 79.06(5) 3_446 2_466 ?
O4 Ca1 Ca3 130.5(2) 3_446 2_465 ?
O1 Ca1 Ca3 139.2(3) . 2_465 ?
O5 Ca1 Ca3 45.2(2) 2_465 2_465 ?
O6 Ca1 Ca3 38.09(19) 2_465 2_465 ?
O4 Ca1 Ca3 84.98(19) 3_445 2_465 ?
O6 Ca1 Ca3 86.6(2) 2_466 2_465 ?
B1 Ca1 Ca3 107.8(2) 2_565 2_465 ?
B2 Ca1 Ca3 83.4(3) 1_456 2_465 ?
Ca3 Ca1 Ca3 93.87(5) 3_446 2_465 ?
Ca3 Ca1 Ca3 57.32(4) 2_466 2_465 ?
O4 Ca1 Ca2 99.45(19) 3_446 . ?
O1 Ca1 Ca2 32.9(3) . . ?
O5 Ca1 Ca2 147.5(2) 2_465 . ?
O6 Ca1 Ca2 89.9(2) 2_465 . ?
O4 Ca1 Ca2 58.76(18) 3_445 . ?
O6 Ca1 Ca2 132.52(19) 2_466 . ?
B1 Ca1 Ca2 53.9(2) 2_565 . ?
B2 Ca1 Ca2 117.83(16) 1_456 . ?
Ca3 Ca1 Ca2 111.50(5) 3_446 . ?
Ca3 Ca1 Ca2 168.99(6) 2_466 . ?
Ca3 Ca1 Ca2 122.82(6) 2_465 . ?
O3 Ca3 O6 102.7(3) 1_554 . ?
O3 Ca3 O3 97.8(3) 1_554 . ?
O6 Ca3 O3 101.4(3) . . ?
O3 Ca3 O4 123.6(3) 1_554 . ?
O6 Ca3 O4 128.3(3) . . ?
O3 Ca3 O4 94.3(3) . . ?
O3 Ca3 O5 89.4(3) 1_554 1_554 ?
O6 Ca3 O5 77.7(3) . 1_554 ?
O3 Ca3 O5 172.7(3) . 1_554 ?
O4 Ca3 O5 80.9(3) . 1_554 ?
O3 Ca3 O5 176.7(3) 1_554 . ?
O6 Ca3 O5 77.4(3) . . ?
O3 Ca3 O5 85.4(3) . . ?
O4 Ca3 O5 55.0(2) . . ?
O5 Ca3 O5 87.4(3) 1_554 . ?
O3 Ca3 B1 148.4(3) 1_554 4_565 ?
O6 Ca3 B1 98.4(3) . 4_565 ?
O3 Ca3 B1 100.7(3) . 4_565 ?
O4 Ca3 B1 29.9(3) . 4_565 ?
O5 Ca3 B1 72.4(3) 1_554 4_565 ?
O5 Ca3 B1 29.1(3) . 4_565 ?
O3 Ca3 O5 54.4(2) 1_554 4_464 ?
O6 Ca3 O5 157.1(3) . 4_464 ?
O3 Ca3 O5 83.2(2) . 4_464 ?
O4 Ca3 O5 73.0(2) . 4_464 ?
O5 Ca3 O5 100.4(2) 1_554 4_464 ?
O5 Ca3 O5 125.52(16) . 4_464 ?
B1 Ca3 O5 102.7(3) 4_565 4_464 ?
O3 Ca3 B1 28.1(3) 1_554 1_554 ?
O6 Ca3 B1 129.9(3) . 1_554 ?
O3 Ca3 B1 85.1(3) . 1_554 ?
O4 Ca3 B1 100.1(3) . 1_554 ?
O5 Ca3 B1 101.1(3) 1_554 1_554 ?
O5 Ca3 B1 152.4(3) . 1_554 ?
B1 Ca3 B1 129.41(18) 4_565 1_554 ?
O5 Ca3 B1 27.4(3) 4_464 1_554 ?
O3 Ca3 O2 67.4(4) 1_554 . ?
O6 Ca3 O2 52.6(3) . . ?
O3 Ca3 O2 69.5(3) . . ?
O4 Ca3 O2 162.4(4) . . ?
O5 Ca3 O2 114.5(3) 1_554 . ?
O5 Ca3 O2 114.8(4) . . ?
B1 Ca3 O2 143.6(4) 4_565 . ?
O5 Ca3 O2 110.4(3) 4_464 . ?
B1 Ca3 O2 85.7(4) 1_554 . ?
O3 Ca3 B2 85.1(3) 1_554 . ?
O6 Ca3 B2 25.6(3) . . ?
O3 Ca3 B2 85.6(3) . . ?
O4 Ca3 B2 150.8(3) . . ?
O5 Ca3 B2 95.9(3) 1_554 . ?
O5 Ca3 B2 96.0(3) . . ?
B1 Ca3 B2 121.5(4) 4_565 . ?
O5 Ca3 B2 135.6(3) 4_464 . ?
B1 Ca3 B2 109.0(4) 1_554 . ?
O2 Ca3 B2 26.9(4) . . ?
O3 Ca3 B1 91.5(3) 1_554 . ?
O6 Ca3 B1 124.9(3) . . ?
O3 Ca3 B1 23.5(3) . . ?
O4 Ca3 B1 79.0(3) . . ?
O5 Ca3 B1 156.4(3) 1_554 . ?
O5 Ca3 B1 91.1(3) . . ?
B1 Ca3 B1 95.4(3) 4_565 . ?
O5 Ca3 B1 61.8(3) 4_464 . ?
B1 Ca3 B1 70.7(2) 1_554 . ?
O2 Ca3 B1 87.5(3) . . ?
B2 Ca3 B1 107.6(4) . . ?
O5 B1 O4 118.2(9) 4_465 4_465 ?
O5 B1 O3 121.7(9) 4_465 . ?
O4 B1 O3 120.1(10) 4_465 . ?
O5 B1 Ca3 70.0(6) 4_465 4_465 ?
O4 B1 Ca3 62.5(5) 4_465 4_465 ?
O3 B1 Ca3 142.4(7) . 4_465 ?
O5 B1 Ca3 73.2(6) 4_465 1_556 ?
O4 B1 Ca3 157.5(7) 4_465 1_556 ?
O3 B1 Ca3 52.1(5) . 1_556 ?
Ca3 B1 Ca3 138.2(4) 4_465 1_556 ?
O5 B1 Ca2 153.0(7) 4_465 . ?
O4 B1 Ca2 81.2(6) 4_465 . ?
O3 B1 Ca2 42.9(5) . . ?
Ca3 B1 Ca2 136.8(4) 4_465 . ?
Ca3 B1 Ca2 82.5(3) 1_556 . ?
O5 B1 Ca3 106.0(6) 4_465 . ?
O4 B1 Ca3 119.6(7) 4_465 . ?
O3 B1 Ca3 42.5(4) . . ?
Ca3 B1 Ca3 101.3(3) 4_465 . ?
Ca3 B1 Ca3 70.7(2) 1_556 . ?
Ca2 B1 Ca3 75.9(3) . . ?
Ho2 O1 Ho2 103.8(6) . 1_556 ?
Ho2 O1 Ho1 112.6(4) . 2_565 ?
Ho2 O1 Ho1 113.3(4) 1_556 2_565 ?
Ca2 O1 Ca1 112.6(4) . . ?
Ho2 O1 Ho1 112.6(4) . . ?
Ho2 O1 Ho1 113.3(4) 1_556 . ?
Ho1 O1 Ho1 101.5(6) 2_565 . ?
O6 B2 O6 119.7(13) . 2_565 ?
O6 B2 O2 120.1(7) . . ?
O6 B2 O2 120.1(7) 2_565 . ?
O6 B2 Ca3 47.5(4) . . ?
O6 B2 Ca3 167.2(9) 2_565 . ?
O2 B2 Ca3 72.6(3) . . ?
O6 B2 Ca3 167.2(9) . 2_565 ?
O6 B2 Ca3 47.5(4) 2_565 2_565 ?
O2 B2 Ca3 72.6(3) . 2_565 ?
Ca3 B2 Ca3 145.1(6) . 2_565 ?
O6 B2 Ca1 99.7(8) . 1_654 ?
O6 B2 Ca1 38.6(6) 2_565 1_654 ?
O2 B2 Ca1 129.1(8) . 1_654 ?
Ca3 B2 Ca1 136.2(5) . 1_654 ?
Ca3 B2 Ca1 70.93(15) 2_565 1_654 ?
B2 O2 Ho2 130.5(12) . . ?
B2 O2 Ca2 130.5(12) . . ?
B2 O2 Ho2 132.4(12) . 1_554 ?
Ho2 O2 Ho2 97.2(5) . 1_554 ?
B2 O2 Ca3 80.5(3) . . ?
Ho2 O2 Ca3 95.5(3) . . ?
Ca2 O2 Ca3 95.5(3) . . ?
Ho2 O2 Ca3 97.1(3) 1_554 . ?
B2 O2 Ca3 80.5(3) . 2_565 ?
Ho2 O2 Ca3 95.5(3) . 2_565 ?
Ho2 O2 Ca3 97.1(3) 1_554 2_565 ?
Ca3 O2 Ca3 160.9(5) . 2_565 ?
B1 O3 Ca3 99.8(6) . 1_556 ?
B1 O3 Ca3 114.1(6) . . ?
Ca3 O3 Ca3 97.8(3) 1_556 . ?
B1 O3 Ca2 113.5(6) . . ?
Ca3 O3 Ca2 118.0(3) 1_556 . ?
Ca3 O3 Ca2 112.3(3) . . ?
B1 O3 Ho2 113.5(6) . . ?
Ca3 O3 Ho2 118.0(3) 1_556 . ?
Ca3 O3 Ho2 112.3(3) . . ?
B1 O4 Ho1 143.5(7) 4_565 3_554 ?
B1 O4 Ho1 108.3(6) 4_565 3 ?
Ho1 O4 Ho1 98.2(3) 3_554 3 ?
B1 O4 Ca3 87.6(6) 4_565 . ?
Ho1 O4 Ca3 96.8(3) 3_554 . ?
Ho1 O4 Ca3 126.1(3) 3 . ?
B1 O5 Ho1 138.8(6) 4_565 2_665 ?
B1 O5 Ca3 121.6(6) 4_565 1_556 ?
Ho1 O5 Ca3 99.0(3) 2_665 1_556 ?
B1 O5 Ca3 80.9(6) 4_565 . ?
Ho1 O5 Ca3 95.6(3) 2_665 . ?
Ca3 O5 Ca3 87.4(3) 1_556 . ?
B1 O5 Ca3 79.4(6) 4_565 4_566 ?
Ho1 O5 Ca3 86.4(2) 2_665 4_566 ?
Ca3 O5 Ca3 120.0(3) 1_556 4_566 ?
Ca3 O5 Ca3 152.0(3) . 4_566 ?
B2 O6 Ca3 106.8(7) . . ?
B2 O6 Ho1 123.8(8) . 2_665 ?
Ca3 O6 Ho1 103.7(3) . 2_665 ?
B2 O6 Ho1 120.2(8) . 2_664 ?
Ca3 O6 Ho1 102.5(3) . 2_664 ?
Ho1 O6 Ho1 97.0(3) 2_665 2_664 ?

